High Energy Rate Forming & Powder Metallurgy . In these forming processes large amount of energy is applied for a very short interval of time.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
In these forming processes large amount of energy is applied for a very short interval of time.
The process has been successfully used to form steel plates 25 mm thick x 4 m diameter and to bulge steel tubes as thick as 25 mm.
Explosive Forming Operations can be divided into two groups, depending on the position of the explosive charge relative to the workpiece.
In this method, the explosive charge is located at some predetermined distance from the workpiece and the energy is transmitted through an intervening medium like air, oil, or water. Peak pressure at the workpiece may range from a few thousand psi to several hundred thousand psi depending on the parameters of the operation.
In this method, the explosive charge is held in direct contact with the workpiece while the detonation is initiated. The detonation produces interface pressures on the surface of the metal up to several million psi (35000 MPa).
A high charging voltage is supplied for a short time to a bank of capacitors connected in parallel.
Magnetic forming can be accomplished in any of the following three ways, depending upon the requirements.
• melting point is too high
• reaction occurs at melting
• too hard to machine
• very large quantity
– Porous bearings and filters
– Very high MP metals (W alloys, WC-Co tools)
– Very highly alloyed metals
Powder metallurgy may be defined as the art of producing metal powders and using them to make serviceable objects.
Components can be made from pure metals, alloys, or mixture of metallic and non-metallic powders
Raw materials => Powder; Powders can be pure elements, pre-alloyed powders
Powders along with additives are mixed using mixers
Lubricants are added prior to mixing to facilitate easy ejection of compact and to minimize wear of tools; Waxes, metallic stearates, graphite etc.
Powder characterization – size, flow, density, compressibility tests
Dies are made of cemented carbide, die/tool steel; pressed using hydraulic or mechanical presses
The basic purpose of compaction is to obtain a green compact with sufficient strength to withstand further handling operations
The green compact is then taken for sintering
It serves to consolidate the mechanically bonded powders into a coherent body having desired on service behavior
1. Mechanical methods,
2. Physical methods,
3. Chemical methods
Milling: During milling, impact, attrition, shear and compression forces are acted upon particles.
During impact, striking of one powder particle against another occurs.
Attrition refers to the production of wear debris due to the rubbing action between two particles.
Shear refers to cutting of particles resulting in fracture. The particles are broken into fine particles by squeezing action in compression force type.
Machining: Mg, Be, Ag, solder, dental alloy are specifically made by machining;
Turning and chips thus formed during machining are subsequently crushed or ground into powders
In this method, the processing conditions are so chosen that metals of high purity are precipitated from aqueous solution on the cathode of an electrolytic cell. This method is mainly used for producing copper, iron powders. This method is also used for producing zinc, tin, nickel, cadmium, antimony, silver, lead, beryllium powders.
at cathode Cu+ + e- -> Cu
1. A hard brittle layer of pure metal which is subsequently milled to obtain powder (eg. iron powder)
2. A soft, spongy substance which is loosely adherent and easily removed by scrubbing
3. A direct powder deposit from the electrolyte that collects at the bottom of the cell
Powders of high purity with excellent sinterability
Wide range of powder quality can be produced by altering bath composition
Time consuming process; Pollution of work place because of toxic chemicals;
Waste disposal is another issue; Cost involved in oxidation of powders and hence they should be washed thoroughly
In conventional (gas or water) atomization, a liquid metal is produced by pouring molten metal through a tundish with a nozzle at its base. The stream of liquid is then broken into droplets by the impingement of high pressure gas or water. This disintegration of liquid stream is shown in fig.
This has five stages
i) Formation of wavy surface of the liquid due to small disturbances
ii) Wave fragmentation and ligament formation
iii) Disintegration of ligament into fine droplets
iv) Further breakdown of fragments into fine particles
v) Collision and coalescence of particles
1. Water atomization: High pressure water jets are used to bring about the disintegration of molten metal stream. Water jets are used mainly because of their higher viscosity and quenching ability. This is an inexpensive process and can be used for small or large scale production. But water should not chemically react with metals or alloys used.
2. Gas atomization: Here instead of water, high velocity argon, nitrogen and helium gas jets are used. The molten metal is disintegrated and collected as atomized powder in a water bath. Fluidized bed cooling is used when certain powder characteristics are required.
3. Vacuum atomization: In this method, when a molten metal supersaturated with a gas under pressure is suddenly exposed into vacuum, the gas coming from metal solution expands, causing atomization of the metal stream. This process gives very high purity powder. Usually hydrogen is used as gas. Hydrogen and argon mixture can also be used.
4. Centrifugal atomization: In this method, one end of the metal bar is heated and melted by bringing it into contact with a non-consumable tungsten electrode, while rotating it longitudinally at very high speeds. The centrifugal force created causes the metal drops to be thrown off outwards. This will then be solidified as spherical shaped particles inside an evacuated chamber. Titanium powder can be made using this technique
5. Rotating disk atomization: Impinging of a stream of molten metal on to the surface of rapidly spinning disk. This causes mechanical atomization of metal stream and causes the droplets to be thrown off the edges of the disk. The particles are spherical in shape and their size decreases with increasing disk speed.
6. Ultrarapid solidification processes: A solidification rate of 1000C/s is achieved in this process. This results in enhanced chemical homogeneity, formation of metastable crystalline phases, amorphous materials.
Powders manufactured for P/M applications can be classified into – elemental powders, and pre-alloyed powders
Elemental powders => powders of single metallic element; eg.: iron for magnetic applications
Pre-alloyed powders => more than one element; made by alloying elemental powders during manufacturing process itself; In this case, all the particles have same nominal composition and each particle is equivalent to small ingot
i) Drying to remove moisture,
ii) grinding/crushing to obtain fine sizes,
iii) particle size classification to obtain the desired particle size distribution,
v) mixing and blending of powders,
vi) lubricant addition for powder compaction,
vii) powder coating
Refers to the removal of contaminants, solid or gaseous, from the powder particles
Solid contaminants => come from several sources like nozzles or crucible linings.
They interfere during compaction and sintering preventing proper mechanical bonding. Most of these contaminants are non-reactive, but they act as sites for crack nucleation and reduce the dynamic properties of the sintered part.
Non-metallic solid impurities can be removed from superalloy powders by particle separators, electrostatic separation techniques
Gaseous impurities like hydrogen and oxygen get into powders during processing, storage or handling if proper care is not taken. Finer the powders, contamination will be more because of large powder surface area.
These gaseous impurities can form undesirable oxides during processing at relatively high temperature or gets trapped inside the material as pores, reducing the in situ performance of the P/M part.
Degassing techniques like cold, hot static or dynamic degassing methods are used to remove adsorbed gases from the powders
Lubricants added to the powders for better compaction has to be removed for desirable final P/M part
b) Grinding: similar to the mechanical methods seen earlier; Milling is widely used for reducing the aggregates of powder.
Milling time, speed, type can be selected for getting required degree of grinding
c) Powder classification & screening: Powder size and shape, size distribution varied within specified range is required for better behavior of P/M parts.
In this method, the desired particle size distributions with particle sizes within specific limits can be obtained. These variation depends on lot also.
d) Blending & mixing: Blending – Process in which powders of the same nominal composition but having different particle sizes are intermingled.
This is done to
(i) obtain a uniform distribution of particle sizes, i.e. powders consisting of different particle sizes are often blended to reduce porosity,
(ii) for intermingling of lubricant with powders to modify metal to powder interaction during compaction
Mixing – process of combining powders of different chemistries such as elemental powder mixes (Cu-Sn) or metal-nonmetal powders.
This may be done in dry or wet condition.
Liquid medium like alcohol, acetone, benzene or distilled water are used as milling medium in wet milling.
Ball mills or rod mills are employed for mixing hard metals such as carbides.
Depending on the extent of mixing, mixing can be classified as
(i) perfectly mixed or uniform mixing,
(ii) random mixed, &
(iii) totally un-mixed.
The mixing should be stopped when random mixture is achieved. Overmixing leads to reduced flow characteristics of the mix.
Heat treatment is generally carried out before mixing or blending the metal powders.
Some of the important objectives are,
i) Improving the purity of powder:
Reduction of surface oxides from powders by annealing in hydrogen or other reducing atmosphere.
Dissolved gases like hydrogen and oxygen, other impurities are removed by annealing of powders.
Lowering impurities like carbon results in lower hardness of the powder and hence lower compaction pressures & lower die wear during compaction.
For eg., atomized powders having a combined carbon and oxygen content as high as 1% can be
reduced after annealing to about 0.01% carbon and 0.2% oxygen.
Heat treatment is done at protective atmosphere like hydrogen, vacuum.
ii) Improving the powder softness:
Aim is to reduce the work hardening effect of powders that has be crushed to obtain fine powders; while many powders are made by milling, crushing or grinding of bulk materials. Powder particles are annealed under reducing atmosphere like hydrogen. The annealing temperature is kept low to avoid fusion of the particles.
iii) Modification of powder characteristics:
The apparent density of the powders can be modified to a higher or lower value by changing the temperature of treatment.
Compaction is an important step in powder processing as it enables the forming of loose metal powders into required shapes with sufficient strength to withstand till sintering is completed.
In general, compaction is done without the application of heat. Loose powders are converted into required shape with sufficient strength to withstand ejection from the tools and subsequent sintering process.
In cases like cemented carbide, hot compaction is done followed by sintering. One can not call this as compaction strictly, as sintering is also involved in this.
Powder compaction methods
Powder compaction techniques can be classified as,
1. Methods without application of pressure –
i) loose powder sintering in mould,
ii) vibratory compaction,
iii) slip casting,
iv) slurry casting,
v) injection moulding
2. Methods with applied pressure –
i) cold die compaction (single action pressing, double action pressing, floating die pressing),
ii) isostatic pressing,
iii) powder rolling,
iv) powder extrusion,
v) explosive compaction
Used for the production of simple and low density parts such as filters, other parts that are porous in nature; these techniques involve no external force and depend upon gravity for powder packing
Loose powder sintering: - Also known as loose powder shaping, gravity sintering, pressureless sintering.
In this method, the metal powder is vibrated mechanically into the mould, which is the negative impression of the product and heated to sintering temperature.
This is the simplest method and involve low cost equipment.
The main reasons for not using this method for part production are, difficulty of part removal from the mould after sintering, & considerable shrinkage during sintering.
Amount of porosity ranges from 40 vol% to 90 vol%;
Highly porous filter materials made of bronze, stainless steel, and monel, porous nickel membrane for use as electrodes in alkaline storage batteries and fuel cells are typical examples.
Slip casting: - Used for compacting metal and ceramic powders to make large & complex shapes for limited production runs.
A slip is a suspension of metal or ceramic powder (finer than 5 m) in water or other soluble liquid which is pored into a mould, dried and further sintered.
i) Preparing assembled plaster mould,
ii) filling the mould,
iii) absorption of water from the slip into the porous mould,
iv) removal of part from the mould,
v) trimming of finished parts from the mould
Sometimes mould release agents like oil, graphite can be used.
Hollow and multiple parts can be produced
Advantages of slip casting:
Products that can not be produced by pressing operation can be made,
No expensive equipment is required,
Works best with finest powder particles
Limited commercial applications
Tubes, boats, crucibles, cones, turbine blades, rocket guidance fins; Also products with excellent surface finish like basins, water closets.
Slurry casting: This process is similar to slip casting except that a slurry of metal powders with suitable liquids, various additives, and binders is poured into a mould and dried. The solvent is removed either by absorption into the POP or by evaporation. Very high porous sheet for use as electrodes in fuel cells and nickel-cadmium rechargeable batteries are produced by this method.
Tape casting (doctor blade casting): This is a variation of slurry casting process and is used to produce thin flat sheets.
This process involves preparing a dispersion of metal or ceramic powder in a suitable solvent with the addition of dispersion agent (to improve the dispersion of the particles). Then a binder is added and fed to a reservoir. Whole mixture is fed on to a moving carrier film from the bottom of the reservoir.
This slurry layer is deposited on the film by the shearing action of a blade. The slurry should be free of air bubbles, otherwise result in porosity. During sintering, the binder is burnt off first and densification of material occurs.
In present days, endless stainless steel belt is used instead of carrier tape. This process can be used for making very thin tapes between 50 to 1000 m thickness. This method is used for making electronic substrates, dielectrics for capacitors and piezoelectric actuators.
Vibratory compaction:Vibratory compaction uses vibration energy to compact the powder mass. During this process, smaller voids can be filled with particles of still smaller size and this sequence is carried out till a high packing density of powder is achieved even before consolidation.
Mechanical vibration facilitates the formation of nearly close packed powder by settling particles in the voids present in the powder agglomerate. During vibration, small pneumatic pressure is usually superimposed on the powder mass.
Brittle powders can be compacted by this method as they develop crack if done by pressure compaction
This method is generally used when,
1) powders have irregular shape,
2) use of plasticizers for forming is not desirable,
3) sintered density is required to be very close theoretical density
Wet bag process:
In this, the mould is directly in contact with the fluid.
This reduces the productivity, since the bag has to be removed every time before refilling.
Tooling costs are reduced in this.
Fixed mould process:
The mould is fixed in the pressure vessel and powders are filled in situ.
The tooling has internal channel into which fluid is pumped.
This is an automated process in which the powder filling, compaction, depressurization and removal of green parts are done continuously.
This involves higher tooling cost, but has higher production rate.
Advantages of CIP:
Uniform, controlled, reproducible densification of powder.
Long, slender parts can be pressed.
Neat net shape forming.
Short production times.
Economy of operation for complex and large parts.
Metallic filters made from bronze, brass, stainless steel, Inconel, Monel, Titanium, high speed tools, carbide tools.
Also ceramic parts such as sparks plugs and insulators are made by this method.
This process involves feeding of powders between rolls to produce a coherent and brittle green strip.
This green strip is then sintered & re-rolled to obtain a dense, finished product.
Nickel strips for coinage, nickel-iron strips for controlled expansion properties, Cu-Ni-Sn alloys for electronic applications, porous nickel strip for alkaline batteries and fuel cell applications.
a) solid state sintering – This is the commonly occurring consolidation of metal and alloy powders. In this, densification occurs mainly because of atomic diffusion in solid state.
b) Liquid phase sintering – The densification is improved by employing a small amount of liquid phase (1-10% vol). The liquid phase existing within the powders at the sintering temperature has some solubility for the solid. Sufficient amount of liquid is formed between the solid particles of the compact sample. During sintering, the liquid phase crystallizes at the grain boundaries binding the grains. During this stage, there is a rapid rearrangement of solid particles leading to density increase. In later stage, solid phase sintering occurs resulting in grain coarsening and densification rate slows down.
Used for sintering of systems like tungsten-copper and copper-tin. Also covalent compounds like silicon nitride, silicon carbide can be made, that are difficult to sinter.
c) Activated sintering – In this, an alloying element called ‘doping’ is added in small amount improves the densification by as much as 100 times than undoped compact samples. Example is the doping of nickel in tungsten compacts
d) Reaction sintering – In this process, high temperature materials resulting from chemical reaction between the individual constituents, giving very good bonding. Reaction sintering occurs when two or more components reacts chemically during sintering to create final part. A typical example is the reaction between alumina and titania to form aluminiumtitanate at 1553 K which then sinters to form a densified product.
Other than mentioned above, rate controlled sintering, microwave sintering, gas plasma sintering, spark plasma sintering are also developed and practiced.